ISSN Online: 2327-6053 ISSN Print: 2327-6045
DOI: 10.4236/msce.2017.59002 Sep. 28, 2017 10 Journal of Materials Science and Chemical Engineering
Results from Multi Technique Investigation of
Pottery from Different Early Neolithic Sites in
, Nikolla Civici1
, Enkeleida Beqiraj3
, Ilir Gjipali4
1Institute of Applied Nuclear Physics, University of Tirana, Tirana, Albania 2Department of Physics, University of Tirana, Tirana, Albania
3Department of Earth Sciences, Polytechnic University of Tirana, Tirana, Albania 4Institute of Archaeology, Centre of Albanian Studies, Tirana, Albania
The archaeological excavations of the Neolithic sites in Albania show that this area has been the center of the confluence of different cultures with various levels of development and social organization. This is reflected in the pottery manufacturing, which during early Neolithic is classified in three major groups. The pottery from the Early Neolithic site at Kolsh, situated in north east, shows similarities with all the other cultures of central Balkans, the shards from the site Blaz in the north-west region show an Adriatic-Mediterraean character, while the south culture represented by Vashtemi and Podgorie sites appears to show cultural report with early Neolithic in the area of Thessaloniki. During the last years, the Institute of Applied Nuclear Physics of the University of Ti-rana and the Institute of Archaeology of the Center of Albanian Studies have initiated a cooperative study of the ceramic finds which aims at a better cha-racterization and classification of the ceramic finds. In this context Optical Microscopy (OM), EDXRF, micro-XRF and XRD were used for the elemental and structural characterization of ceramic samples. Some data on the fabric texture, inclusions, decoration materials and elemental composition of the shards from pottery samples belonging to the mentioned Early Neolithic sites in Albania will be presented.
Neolithic Ceramics, EDXRF, Micro-XRF, Albania
Analysis of pottery from excavations involves two main lines of inquiry. The first, How to cite this paper: Ndreçka, E., Civici,
N., Beqiraj, E. and Gjipali, I. (2017) Results from Multi Technique Investigation of Pot-tery from Different Early Neolithic Sites in Albania. Journal of Materials Science and Chemical Engineering, 5, 10-26.
Received: July 25, 2017 Accepted: September 25, 2017 Published: September 28, 2017
Copyright © 2017 by authors and Scientific Research Publishing Inc. This work is licensed under the Creative Commons Attribution International License (CC BY 4.0).
DOI: 10.4236/msce.2017.59002 11 Journal of Materials Science and Chemical Engineering termed typological analysis consists chiefly of detailed analysis of the rim forms and decorative features of vessels. The other line of inquiry involves the exami-nation of pottery fabrics—the aim here being to determine the raw materials and processes used in the manufacture of pottery. The results of both fabric analysis and typological analysis can then be combined to establish definitive pottery styles which will help in the interpretation of archaeological excavation.
While the typological study of the pottery is widely used by the archaeologists in Albania, only a few studies related with pottery materials and their production technology are published   . The main objective of the present study is the collection of data for the materials (clay composition and pigments) and tech-nology (tempers and firing conditions) used for the manufacture of pottery ex-cavated at the different early Neolithic sites and based on them to find similari-ties and/or differences that can be useful for better archaeological classifications. In this context different X-ray techniques EDXRF (Energy Dispersive X-ray Fluorescence), Micro-XRF (Micro X-ray fluorescence), XRD (X-ray diffraction), Optical Microscopy together with various multivariate techniques are being used for the characterization of the raw materials and investigation of the technologies used for the production of ceramic finds from different sites in Albania. EDXRF spectrometry was employed for the determination of the chemical composition of the pottery. The evaluation of the chemical data through simple elemental bip-lots and their treatment by means of multivariate statistical analysis (CA) led to the potential classification of the samples into distinctive groups and provided feedback for further discussion about their provenance. OM, XRD and µ-XRF were used for the investigation of the internal texture of the ceramic body and identification of the major types of inclusions as well as the materials used for the external decorations.
2. Archaeological Background
The geographical position of Albania, at the intersection of land routes that con-nect Anatolia, the Balkans and the Western Mediterranean on one side and its long Adriatic and Ionian coast on the other side, has determined the cultural features of its Neolithic civilization which combines elements of the Anatolian-Balkan and Adriatic-Mediterranean cultural complexes .
Pottery manufacturing during early Neolithic in Albania is classified in two major groups: north culture represented by Kolshi and Blazi sites and south cul-ture represented by Vashtëmi-Podgorie sites (Figure 1).
DOI: 10.4236/msce.2017.59002 12 Journal of Materials Science and Chemical Engineering
Figure 1. The distribution of Neolithic cultures in Albania.
DOI: 10.4236/msce.2017.59002 13 Journal of Materials Science and Chemical Engineering dates in Vashtëmi place it within the first wave of Early Neolithic settlements in the Korça basin. This recent study dates Vashtemi between 6470-6370 cal BC and Podgori between 6070-5970 cal BC .
The Blazi cave settlement, located in Mati river valley in northeast of Albania, was excavated by F. Prendi and Zh. Andrea from 1978 to 1979. Blazi early lithic culture shows special features that tie it with Adriatic group of Early Neo-lith. Blazi ceramics is characterized by coarse pottery, with grey, black or brown burnished exterior and predominantly Impresso type of decorations  .
Kolshi culture was excavated in 1974 due to some superficial findings from an expedition in Kukësi area. Kolsh ceramics is mainly with thick walls, with brown or reddish colour and barbotine decorations. The amount of fine ceramics is rel-atively small, and appears in carefully modeled shapes, with small dimensions and thin walls. The sherds from Kolsh are decorated with geometric motifs of red or dark brown colors on red background. The Kolsh culture shows similari-ties and connections with the culture of central Balkans  .
Although these cultures sprang from different origins, they were not isolated in their development but on the contrary entered into close contact with one another. This may be seen in the interchange of cultural elements, those of east Albania appearing in west Albania and vice versa; for example, the Barbotine pottery of Starcevo appearing in Blaz II, or “impress” pottery of Adriatic type at Vashtemi  .
3. Samples and Sample Preparation
We will consider here a small group of pottery shards from the collection of the excavations at four early Neolithic sites in Albania. The sites named Vashtemi and Podgori are situated in south east of Albania, while the sites named Kolsh and Blaz are situated respectively in the northeastern and northwestern part of the country. 20 - 30 shards from each site were selected by the archaeologists and we were allowed to cut small pieces and use them for the analysis. The shards from all the sites belong to pottery with thick and thin walls (Figure 2). Most of the shards show dark red and black color with black layers in the middle and some of them are painted on the surface.
Fresh cross sections of some of the shards were polished on successive grades of grinding paper (silicon carbide) and after cleaning and drying were used for optical microscopy and micro-XRF examinations. Standard thin sections have been prepared from the ceramic shards for the mineralogical and petrographic characterization.
DOI: 10.4236/msce.2017.59002 14 Journal of Materials Science and Chemical Engineering
Figure 2. Ceramic shards from the studied sites.
from the same fine powder, placed in the sample holder with a flat surface, was used for XRD analysis in reflection mode.
4. Analytical Techniques
The microscopic petrographic investigations were carried out on a Leitz Labor-lux 11 Pol S polarizing microscope.
DOI: 10.4236/msce.2017.59002 15 Journal of Materials Science and Chemical Engineering the elements in the spectra. Areas up to 10 mm2 with spatial resolution of 0.1 mm were scanned in 5 - 6 hours.
The elemental composition of the samples was determined by EDXRF spec-trometry. Two different EDXRF systems were used for the effective excitation of more than 20 elements in each sample. Elements from K to Zr were excited by a Mo secondary target and the 59.6 keV radiation of Am-241 source was used to excite the K lines of some heavier elements (Ba - Nd). The first system that uses the sec-ondary target excitation mode, consists of a Philips 1729 X-ray generator equipped with Mo anode X-ray tube (max. 50 kV *40 mA); a 30 mm2 Canberra Si(Li) de-tector, while the second system is based on 30 mCi Am-241 excitation source and 80 mm2 PGT HpGe detector. Both systems use a 900 source-sample-detector geometry and similar pulse processing chains consisting of Canberra spectros-copy amplifier (Mod. 2024), ADC (Mod. 8706), S-100 and Accuspec B MCA cards installed on separate PC-s and Gennie 2000 software. Thin Mo and Pb foils were respectively used for filtering the scattered radiation and the low energy lines of the Am source in each of the systems. The operating conditions of each measurement are presented in Table 1.
The intensities of the analytes’ line were calculated by the program AXIL . An approximate sample composition, peak shape correction together with the other required parameters were included in the fitting model. The program COREX , which uses back scattered peaks and fundamental parameters, was used for the calculation of the concentrations of the elements excited by Mo secondary target. A set of about 40 “calibrators” prepared from pure elements and or com-pounds were measured in the same conditions and the results were used for the required experimental calibrations (Excitation-detection efficiency vs atomic num-ber, mass absorption coefficient at Compton energy vs the intensity of Compton Peak and average atomic number of sample vs the ratio of the scattered peaks). The concentrations of Ba, La, Ce and Nd, excited by the Am-241 source, were calculated using the Compton scattered peak as internal standard . As the composition of ceramic samples are generally similar to that of soils and ments, a series of sediment reference materials (GSD1-12, Chinese stream sedi-ment SRM-s , IAEA standards SL-1, Soil-5 and Soil-7 ) were used for ca-libration in this case.[image:6.595.205.540.666.732.2]
In these conditions we could detect more than 20 elements in each ceramic sample. The calculated values of detection limits for the elements excited by the Mo secondary target vary from 150 - 100 mg/kg for K and Ca, 40 - 15 mg/kg for elements Ti - Fe and 4 - 12 mg/kg for Ni - Zr. The elements excited by Am-241
Table 1. Operating conditions of EDXRF measurements.
Elemental range Source Filter kV/mA Time (s)
K - Zr Mo sec. target Mo 35/20 1500
DOI: 10.4236/msce.2017.59002 16 Journal of Materials Science and Chemical Engineering source show values of detection limits in the range 8 - 10 mg/kg. The precision of the procedure was evaluated by repeated measurements of the Standard Ref-erence Material GSS-1 (Chinese soil SRM) , which was frequently measured together with the samples. From the data summarized in Table 2 it can be seen that the relative standard deviations for major elements are better than 5%, while for minor elements it is generally within 15%, except for some elements that suffer line interferences, blank subtraction or have concentrations close to detec-tion limit. The good agreement between the certified and the calculated concen-trations for this standard is an indication of the good accuracy of the analytical procedure. Additional information about the EDXRF system and the analytical parameters of the procedure can be found elsewhere  .[image:7.595.201.539.315.739.2]
PANALYTICAL XPERT-PRO MPD PW diffractrometer was used for X-Ray diffraction analysis of some of the pottery samples. It is an X-ray computer con-trolled diffractometer system, having a fixed tube Cu target, secondary graphite
Table 2. Reproducibility of the determinations.
Element GSS-1 Calculated
Certified Average St Dev Rel St Dev (%)
K (%) 2.150 2.156 0.087 4.2
Ca (%) 1.230 1.181 0.045 4.0
Ti (%) 0.483 0.462 0.022 5.0
Fe (%) 3.630 3.675 0.053 1.5
V 86.0 102.7 25.7 26.3
Cr 62.0 66.7 11.9 18.7
Mn 1760.0 1750.7 48.2 2.9
Ni 20.4 23.4 4.4 19.7
Cu 20.9 24.5 5.5 22.7
Zn 680.1 672.8 15.8 2.5
Ga 19.3 17.8 1.9 11.4
As 33.5 32.7 5.5 17.7
Rb 140.0 143.7 1.8 1.3
Sr 155.0 162.7 2.3 1.5
Y 24.9 25.8 1.3 5.3
Zr 245.0 244.4 12.1 5.2
Pb 98.0 108.9 5.3 5.1
Th 11.6 11.2 1.2 11.7
Ba 590.0 585.5 7.4 1.3
La 34.0 30.4 4.5 14.5
Ce 70.0 67.1 2.1 3.3
DOI: 10.4236/msce.2017.59002 17 Journal of Materials Science and Chemical Engineering monochromator, flat plate horizontal sample holder and X-Celerator for the faster acquisition of data. The diffractogram patterns were obtained by conti-nuous scanning from 7.5 o – 90 o as 2θ angle. Angle step size is 0.013 o and step time is 30 seconds. It was operated at 40 kV and 40 mA with a source of CuKα radiation of wavelength λ = 1.5405 Å.
The Windows based software package IDAS , which includes Hierarchical Cluster Analysis (HCA) and other multivariate methods, was used for data processing. HCA included in IDAS uses Euclidian distance as dissimilarity measure and mini-mum variance (Ward’s method) as clustering strategy. Centered log ratio trans-formation was applied to the concentration data .
5. Results and Discussions
5.1. Mineralogical Composition
A small number of samples (3 - 4) from each site were investigated for their mi-neralogical composition using thin section petrography and X-ray diffraction. From each group we selected samples with different chemical composition.
The colour of the ceramic body varies from reddish-yellow to brown or red-dish-brown. In cross section, the ceramic wall presents in general a bilayered texture, marked by an outer layer with lighter colour and an inner layer with darker colour (Figure 3). According to Rye , this type of structure can be due to firing in reducing conditions with an oxidizing cooling stage, or to firing organic matter-rich clays in oxidizing conditions. In either of these cases, it is difficult to judge the firing condition by naked eye observation of the paste col-ors.
The thin section petrographic examinations show that generally the fabric of the ceramic body is made of semifine clays with amorphous-microcrystalline structure and contains several voids with spherical and elliptical shape as well as different natural non-plastic inclusions, which belong either to the raw materials or were added as temper (Figure 4). The grains of the inclusions are generally angular to sub-angular and range from 1 - 3 mm in size. They constitute 10% - 15% of the volume in the shards from Kolsh and Blazi and about 5% in the sherds from Vashtemi and Podgorie.[image:8.595.64.538.609.710.2]
In the shards from Kolsh and Blaz the non-plastic inclusions are mainly com-posed of quartz, plagioclase, mica (muscovite), clinopyroxene, calcite and opaque
DOI: 10.4236/msce.2017.59002 18 Journal of Materials Science and Chemical Engineering (a) (b) (c) (d)
Figure 4. Thin section micrograph of Pod Nr. 813 (a), (b), Blaz Nr. 44 (c), (d). Images taken in plane polarized light and in cross-polarized light (PPL, XPL, ×10).
minerals represented by hematite, while those form Vashtemi and Podgorie are mainly composed of quartz, plagioclase, mica (muscovite). Small potsherds and vegetal remnants (transformed into carbon) were also identified in some of the shards from each group.
X-ray maps obtained by micro-XRF spectrometer on a small area (10 - 15 mm2) of the cross section of some shards allow an approximate identification of some of the mineral inclusions in the respective clays. Intensity distribution maps (Figure 5) show the presence of Si, K, Ca and Fe rich particles, which can indicate the presence of the minerals rich in those elements, like silicates, calcite, K-feldspars, hematite, etc.
A limited number of samples from Vashtemi, Podgori, Blaz and Kolsh and the raw clays collected in the area of Vashtemi and Podgori were investigated with X-ray diffraction for the identification of main mineral phases (Figure 6).
The data collected are summarized in Table 3. These data show that quartz and albite are the main mineral phases observed in the shards for Vashtemi and Podgori, while in the shards from Blaz and Kolsh in addition to them calcite, diopsite and hematite are also identified. This is in accordance with thin section petrographic results where clinopiroxen, calcite and hematite were observed among the non plastic inclusions of the shards from Blaz and Kolsh. This should be related with the different geological formations of the areas where the sites are located.
5.2. Elemental Composition
As was previously stated we have analyzed by EDXRF 96 ceramic shards from the Early Neolithic sites of Vashtemi, Podgori, Kolsh and Blaz. In each sample we have determined around 20 elements that include both major and minor elements.
The samples from each site were considered as a separate group and the range of concentrations for each element in the samples from each site are presented in Table 4.
DOI: 10.4236/msce.2017.59002 19 Journal of Materials Science and Chemical Engineering[image:10.595.210.534.276.404.2]
Figure 5. X-ray intensity distribution maps from the cross sections of some shards.
Figure 6. XRD spectra of two representative samples from Blaz and Vashtemi.
Table 3. The main mineral phases identified by XRD.
Quartz Calcite Hematite Albite Diopsite
P-CLAY + + +
Podgori T 1110 + +
Podgori T 700 + +
Podgori H 1230 + +
Podgori H 1343 + +
V-CLAY + +
Vashtemi T 2 + +
Vashtemi T 11 + +
Blazi H 57 + +
Blazi H 189 + +
Blazi T 88 + + + +
Blazi T 227 + + + +
Kolsh T 427 + + +
Kolsh T 1179 + + + +[image:10.595.204.538.455.739.2]
DOI: 10.4236/msce.2017.59002 20 Journal of Materials Science and Chemical Engineering
Table 4. The concentration range of the elements analyzed in the shards from each site. Concentrations in (mg/kg) unless otherwise indicated.
Vashtemi Podgorie Kolsh Blazi
31 20 22 23
Min Max Min Max Min Max Min Max K2O (%) 1.28 2.55 1.50 2.82 0.37 3.50 0.80 3.19 CaO (%) 1.72 3.73 1.95 5.14 1.19 8.39 0.66 17.85 TiO2 (%) 0.65 0.99 0.65 1.05 0.11 0.89 0.14 1.00 Fe2O3 (%) 6.29 10.86 5.20 9.13 6.27 14.72 6.94 22.58
Cr 134 1351 81 495 83 1762 136 6334
Mn 592 1233 305 2441 685 1938 196 2946
Ni 96 476 47 477 163 1004 78 1074
Cu 13 36 6 37 33 199 7 97
Zn 95 146 64 148 63 146 63 169
Ga 7 26 13 28 4 29 4 32
Rb 75 130 81 188 15 131 24 118
Sr 170 278 107 402 46 236 14 95
Y 23 54 23 51 5 34 5 34
Zr 120 309 129 292 47 257 47 235
Ba 702 1153 439 942 148 1052 87 348
La 11 32 14 52 5 22 5 23
Ce 45 80 48 98 9 61 9 60
Nd 14 34 17 38 7 28 7 27[image:11.595.63.541.113.587.2]
Figure 7. Bivariate plots of Fe - Ca and Zr - Sr of all the samples.
DOI: 10.4236/msce.2017.59002 21 Journal of Materials Science and Chemical Engineering looks different for the shards from Kolsh and Blaz where respectively 45% and 60% of the shards are made of calcareous clays (CaO > 5%).
Concerning the Fe2O3 concentration in the body paste of the samples, it is ob-vious from Figure 7(a) and Table 4 that in the samples from Blaz it varies in a much wider range compared with the other groups. Its concentration is quite high in one sample from Kolsh and 5 samples from Blaz.
Bivariate plots of different major and minor elements indicate that most of the shards from Vashtemi and Podgori constitute rather compact groups although there are a few shards which can be considered as outliers from each group (Figure 7). It is worth noticing that in most of the cases the between group differences are not so large and the groups overlap but for some elements there exist ob-servable differences of the concentration ranges of samples from different sites which can constitute evidence that different clay sources may have been used for these wares (Figure 7(b)). The situation appears different for the shards from Kolsh and especially Blaz where the concentrations of the elements vary in a wider range suggesting a quite frequent change of raw materials or different provenance of the pots.
A multidimensional data set consisting of 96 samples (rows) and 18 elements (columns) was created, demanding a multivariate statistical interpretation in order to extract the maximum useful archaeometric information. Hierarchical Cluster Analysis (HCA), specified earlier, was applied to the data matrix. It is worth mentioning that analytical variability, as presented in Table 2, doesn’t in-fluence the HCA results. In test runs of the HCA we included in the data set the results of one clay sample that was measured several times together with the sam-ples and we found out that these artificial samsam-ples were always clustered together in the same cluster without affecting the general cluster structure.
HCA results with five clusters offers an acceptable resolution of the shards from different sites. The dendrogram in Figure 8 shows that the maximum dissimi-larity is observed between the majority of the shards grouped in clusters C3, C2 and C5 and the samples grouped in clusters C1 and C4.
DOI: 10.4236/msce.2017.59002 22 Journal of Materials Science and Chemical Engineering (a) (b)[image:13.595.58.538.65.423.2]
Figure 8. Results of the hierarchical cluster analysis; dendrogarm, cluster population and cluster composition.
The presence of clusters C4 and C5 could indicate local production with differ-ent raw materials (clays and/or temper), while the similarities of a big number of shards with those from the sites of Kolsh and Podgorie could indicate commer-cial connections with those sites.
In conclusion we can state that separate clay deposits, close to each site, have been used for local ceramic production in the sites of Vashtemi, Podgorie and Kolsh. The variability of the chemical composition of the shards from Blaz sup-ports both the local production and the import from other sites. We also observe that in each site the shards with thin and thick walls are clustered together, which means that they are manufactured using the same type of raw materials. The inclusion in the cluster C2 (group of Podgori) and C3 (group of Vashtemi) of a few shards from other sites could be an indication of the exchanges that could have been exiting between the sites. However, more research is needed to fully support this hypothesis.
DOI: 10.4236/msce.2017.59002 23 Journal of Materials Science and Chemical Engineering sherds from Podgori are mostly painted with white color on red background but one of the sherds is painted with bright red color, while the sherds from Kolsh are decorated with red or dark brown colors on red background. Generally the examined shards from Blaz and Vashtemi have not visible coloured decorations, although we have identified the remains of white colour on a shard from Blaz and those of brown colour on a shard from Vashtemi.
Initially the identification of the pigments used for the decorations were per-formed by comparing the micro-XRF spectra measured at the ceramic body with those from the colored areas, but later we thought that X-ray mapping of small areas from the decorated part of the ceramic could give better results. In this way we can clearly observe the variations of the intensity of different elements and connect the pigment with the respective “key elements”.
Some typical examples of the examined decorations are presented in Figure 9.
In Figure 9(a) and Figure 9(b) are presented the results from the dark brown
decorations of a shard from Kolsh and the remains of such a decoration of a shard from Vashtemi. The increased intensities of Mn and Fe in these decora-tions indicate the use of manganese rich pigments (some kind of brown earth). From Figure 9(c) it can clearly be observed that the white part of the decoration is rich in Ca while the red part is rich in Fe, which indicates the use of calcium white (probably calcite) and iron rich material (some kind of red ochre) for the white and red colours of the shards from Podgori. The increased Fe intensity of the red decorated area of the shard compared to the ceramic body indicates that the red colour is due to the application of a pigment and not any kind of red slip. In most of the shards we have found black spots or small areas with black colour which are rich in Ca and P. According to literature data they should be conta-minations related with the environmental conditions of burial  .
Similar types of pigments were identified in studies of Neolithic ceramics from other areas in Balkans and Europe. Calcite, iron oxides and iron and man-ganese compounds (magnetite and jacobsite) were identified in the respective white, red and black pigments used to decorate Cucuteni Neolithic ceramics  as well as the Neolithic ceramics from North Greece . Red ochre and soot were identified in the red and black decorations of the Neolithic ceramics from Slavonia, Croatia , while iron minerals haematite and maghemite were iden-tified in the red decorations of the Neolithic ceramics from southern Spain, the later being an indicator of the firing conditions .
The investigation of ceramic finds from the Neolithic sites of South East Albania with different analytical techniques reveals interesting information regarding the materials and the technology used for their manufacture.
DOI: 10.4236/msce.2017.59002 24 Journal of Materials Science and Chemical Engineering (a)[image:15.595.63.542.71.404.2]
Figure 9. Comparison of X-ray spectra from the ceramic body and decorated areas and respective X-ray intensity distribution maps from the decorated surfaces of some shards from Kolsh (a), Vashtemi (b), Podgori (c).
differences, probably related with the geological formations of the respective areas, were observed in the mineralogical composition of the shards.
Separate clay deposits close to each site should have been used for ceramic production in Vashtemi, Podgori and Kolsh, while the variability of the chemical composition of the shards from Blaz supports both the local production and the import from other sites.
The examination of decorated sherds mostly from the sites of Kolsh and Pod-gori revealed that Ca-rich minerals (probably calcite), Fe-rich minerals (red ochre) and Mn-rich minerals (brown earth) were used respectively for the white, red and brown colours. It should be mentioned that similar types of pigments were found by other researchers on the Neolithic ceramics from different sites in Bal-kan and Europe.
DOI: 10.4236/msce.2017.59002 25 Journal of Materials Science and Chemical Engineering
 Civici, N. (2007) Analysis of Illyrian Terracotta Figurines of Aphrodite and Other Ceramic Objects Using EDXRF Spectrometry. X-Ray Spectrometry, 36, 92-98.
 Ruzi, E (2013) Investigating Compositional Variability among Early Neolithic Ce-ramics from Korça Region, Albania. Chronika, Institute for European and Mediter-ranean Archaeology, 3, 1-15.
 Prendi, F. and Bunguri, A. (2013) The Prehistory of Albania. Institute of Archaeo-logy, Tirana, Albania
 Boardman, J., Edwards, I.E.S., Hammond, N.G.L. and Sollberger, E. (2008) The Prehistory of the Balkans, and the Middle East and the Aegean World, Tenth to Eighth Centuries B.C. In: Boardman, J., Edwards, I.E.S., Hammond, N.G.L. and Sollberger, E., Eds., The Cambridge Ancient History, Vol. III, Part I, 2nd Edition, Cambridge University Press, Cambridge, 187-207.
 Allen, S.E. and Gjipali, I. (2013) New Light on the Early Neolithic in Albania: The Southern Albania Neolithic Archaeological Project (SANAP) 2006-2013. Proceed-ings of the International Congress of Albanian Archaeological Studies, 65th Anni-versary of Albanian Archaeology, Tirana, 21-22 November 2013, 107-120.
 Van Espen, P., Nullens, H. and Adams, F. (1977) A Computer Analysis of X-Ray Fluorescence Spectra. Nuclear Instruments and Methods, 142, 243-250.
 Orlic, I., Makjanic, J., Ross, J. and Valkovic, D. (1988) A General Way of Solving Ma-trix Effect Problems in Elemental Analysis by EDXRFS. X-RaySpectrom, 17, 139-143.
 Anderman, G. and Kemp, J.W. (1958) Scattered X-Ray as Internal Standarts in X-Ray Emission Spectroscopy. Analytical Chemistry, 30, 1306.
 Potts, P.J., Tindle, A.G. and Webb, P.C. (1992) Geochemical Reference Materials Compositions. Whittles Publishing, London.
 IAEA AQCS (2002-2003) Reference Materials Catalogue.
 Civici, N. and Van Grieken, R. (1997) Energy Dispersive X-Ray Fluorescence Anal-ysis in Geochemical Mapping. X-Ray Spectrometry, 26, 147-152.
 Ndreçka, E., Vataj, E., Dilo, T., Gjipali, I. and Civici, N. (2014) Application of EDXRF Spectrometry for the Analysis of Ancient Ceramics. 2nd International Confe-rence on Radiation and Dosimetry in Various Fields of Research, Nis, Serbia, 24-26 May 2014.
 Bondarenko, I., Treiger, B., Van Grieken, R. and Van Espen, P. (1996) Spectrochim.
Electrochimica Acta, 51B, 441.
 Aitchison, J. (1986) The Statistical Analysis of Compositional Data. Chapman and Hall, London, 416 p.https://doi.org/10.1007/978-94-009-4109-0
 Rye, O.S. (1981) Pottery Technology: Principles and Reconstruction. Taraxacum, Washington.
 Tite, M.S. (2008) Ceramic Production, Provenance and Use—A Review. Archaeo-metry, 50, 216-231.
DOI: 10.4236/msce.2017.59002 26 Journal of Materials Science and Chemical Engineering
 Maritan, L. and Mazzoli, C. (2004) Phosphate in Archaeological Finds: Implications for Environmental Conditions of Burial. Archaeometry, 46, 673-683.
 Bugoi, R., Constantinescu, B., Pantos, E. and Popovici, D. (2008) Investigation of Neolithic Ceramic Pigments using Synchrotron Radiation X-Ray Diffraction. Powder Diffraction, 23, 195-199.https://doi.org/10.1154/1.2958068
 Papadopouloua, D., Sakalisa, A., Merousisc, N. and Tsirliganis, N.C. (2007) Study of Decorated Archeological Ceramics by Micro X-Ray Fluorescence Spectroscopy.
Nuclear Instruments and Methods in Physics Research A, 580, 743-746.
 Lukačevića, I. and Rajković, D. (2015) Non-Invasive Analyses of Ancient Ceramics Colorants. Croatica Chemica Acta, 88, 53-58.https://doi.org/10.5562/cca2516
 Capela, J., Huertas, F., Pozzuoli, A. and Linares, J. (2006) Red Ochre Decorations in Spanish Neolithic Ceramics: A Mineralogical and Technological Study. Journal of Archaeological Science, 33, 1157-1166.
Submit or recommend next manuscript to SCIRP and we will provide best service for you:
Accepting pre-submission inquiries through Email, Facebook, LinkedIn, Twitter, etc. A wide selection of journals (inclusive of 9 subjects, more than 200 journals)
Providing 24-hour high-quality service User-friendly online submission system Fair and swift peer-review system
Efficient typesetting and proofreading procedure
Display of the result of downloads and visits, as well as the number of cited articles Maximum dissemination of your research work